observation of wavelength-dependent brewster angle shift in 3d photonic crystals...
Post on 26-Jul-2020
Embed Size (px)
Observation of wavelength-dependent Brewster angle shift in 3D
Priya and Rajesh V. Nair∗
Laboratory for Nano-scale Optics and Meta-materials (LaNOM)
Department of Physics, Indian Institute of Technology (IIT), Ropar
Rupnagar, Punjab 140 001 INDIA ∗Email: firstname.lastname@example.org
The interaction of polarized light with photonic crystals exhibit unique features due to its sub-wavelength nature
on the surface and the periodic variation of refractive index in the depth of the crystals. Here, we present a
detailed study of polarization anisotropy in light scattering associated with three-dimensional photonic crystals
with face centered cubic symmetry over a broad wavelength and angular range. The polarization anisotropy
leads to a shift in the conventional Brewster angle defined for a planar interface with certain refractive index.
The observed shift in Brewster angle strongly depends on the index contrast and lattice constant. Polarization-
dependent stop gap measurements are performed on photonic crystals with different index contrast and lattice
constants. These measurements indicate unique stop gap branching at high-symmetry points in the Brillouin
zone of the photonic crystals. The inherited stop gap branching is observed for TE polarization whereas that is
suppressed for TM polarization as a consequence of Brewster effect. Our results have consequences in the
polarized light-scattering from plasmonic structures and dielectric meta-surfaces and are also useful in
applications like nano-scale polarization splitters and lasers.
Keywords: Photonic crystals, diffraction and scattering, metamaterials, polarization,
The polarization of light is a peculiar property which is inherited from the vectorial nature of wave
equation that governs the light propagation in material media . The polarization of light is defined
as the orientation of associated electric (or magnetic) field with respect to the plane of incidence. It is
possible to decompose the incident light polarization into two orthogonal components and discern the
optical properties based on it. When the electric field is oriented perpendicular to the plane of
incidence, it is called the transverse electric (TE) polarization and when the electric field is oriented
parallel to the plane of incidence, it is called the transverse magnetic (TM) polarization. The
reflectivity and transmittance of light at the planar interface are described on the basis of angle and
polarization state of incident light. A set of equations can be derived for the reflection and transmission
coefficients by satisfying the boundary conditions for electric and magnetic fields at the interface. This
set of equations are specified according to the angle of incidence (θ), polarization state of light, and the
difference in refractive index are known as Fresnel equations . This equation suggests that the
reflectivity increases with increase in θ for TE polarized light. However, in the case of TM
polarization, the reflectivity decreases first, reaches a minimum value at a certain value of θ, and
thereafter it increases. It is interesting to note the zero reflectivity for TM polarization at particular
value of θ known as the Brewster angle (θB) which depends on the ratio of refractive index of the two
materials. The predictions of Fresnel equations are proved subsequently in many isotropic materials
which results in many applications in designing thin film filters, multi-channel filters, polarizers, and
Brewster mirror windows . These polarization-dependent optical phenomena are studied and
explored for applications considering smooth planar semi-infinite isotropic dielectric materials .
Contemporary research interest in the field of nanophotonics has introduced the artificially tailored
dielectric materials on the optical wavelength scale called the photonic metamaterials. The Brewster
effect was originally interpreted for a homogeneous medium howbeit it now encounters an
inhomogeneity at the material interface which entails a modification in the traditional Brewster law for
photonic metamaterials [4, 5]. Recent advances in nano-fabrication techniques shows a great
possibility in the synthesis of photonic metamaterials with exotic optical properties which are
otherwise absent in conventional systems . Photonic crystals are a class of metamaterials wherein
the dielectric constant is varied periodically in either two- or three-orthogonal directions [7, 8]. These
are generally characterised by direction- and polarization-dependent frequency gaps known as
photonic stop gaps wherein certain frequencies of light are forbidden to propagate inside the crystal
. The stop gap arises due to the Bragg diffraction of light from the crystal planes in the propagation
direction. The careful design of the crystal symmetry with appropriate choice of refractive indices,
direction- and polarization-independent frequency gaps are observed called photonic band gap .
The consequence of photonic band gap is the rigorous modification of photon density of states in a
finite frequency range which affect the fundamental properties of light-matter interactions and have
applications in nano-lasers , quantum electrodynamics , and waveguides .
There are other interesting symmetry-dependent optical processes that occur in two- and three-
dimensional photonic crystals are the sub-Bragg diffraction  and stop gap branching [15-17].
These occur when the incident wave vector passes through certain high-symmetry points in the
Brillouin zone of the crystal. The photonic crystals with different symmetry can be synthesized using
various approaches like colloidal self-assembly , laser-writing , and reactive ion-etching 
methods. Among these, self-assembly approach is more attractive for the synthesis of 3D photonic
crystal due to its ease of fabrication and affordability . Such 3D photonic crystals using colloids
with sub-micron diameters are always assembled in the face centered cubic (fcc) symmetry .
The synthesis and optical characterization of 3D self-assembled photonic crystals with fcc symmetry is
well-documented in literature . It has been discussed that self-assembled photonic crystals do not
exhibit a 3D band gap rather possess only photonic stop gaps . Recent interest in the angle- and
polarization-resolved stop gaps indicate interesting optical effects like stop gap branching, band
repulsion, and inhibition of spontaneous emission [23-29]. It is shown that TE polarized light interacts
strongly with the photonic crystal structure and results in stop gap branching whereas it is absent for
TM polarized light due to prevailing Brewster effect . A detailed study of polarization-induced
stop gap formation has shown a direction- and wavelength-dependent shift in θB at the stop gap
wavelength as compared to the conventional definition of θB . Hence there is polarization
anisotropy in the light scattering in photonic crystals. However, the influence of dielectric contrast and
the role of material refractive index dispersion on polarization anisotropy are yet to be analyzed.
In the present work, we investigate the role of index contrast and the wavelength dispersion of material
refractive index on the polarization anisotropy in photonic crystals. We discuss the shift in θB as a
function of index contrast. Further, we elucidate the polarization-dependent stop gap branching for
photonic crystal in different spectral ranges and for different index contrasts. The present study will
amplify the knowledge about strong interaction of polarized light with photonic crystals leading to
multiple prospects in photonics and plasmonics. Additionally, the eccentric Brewster effect in sub-
wavelength nanophotonic structures has its impact in various applications giving them a new edge with
enticing properties, relevant to the polarization of light.
II. Experimental details
IIA. Sample details
The photonic crystals used in the present work are synthesized using convective self-assembly method
. A clean glass substrate is placed vertically in a cuvette containing colloidal suspension of
appropriate volume and concentration which is kept inside a temperature controlled oven for 4-5 days.
It is well-known that self-assembled photonic crystals grown using sub-micron spheres are always
organized into fcc geometry as it is the minimum energy configuration . We have chosen photonic
crystal samples made of polystyrene (PS) microspheres of diameter 803 ± 20 nm (sample A) and 287 ±
8 nm (sample B) to study the role of refractive index dispersion in the origin of polarization anisotropy.
Also samples are grown using polymethyl methacrylate (PMMA) microspheres of diameter 286 ± 10
nm (sample C) to study the impact of index contrast on the polarization anisotropy in photonic crystals
having similar lattice constants.
IIB. Measurement details